Linking Microstructural Evolution and Macro-Scale Linking Microstructural Evolution and Macro-Scale
Embed Size (px)
Transcript of Linking Microstructural Evolution and Macro-Scale Linking Microstructural Evolution and Macro-Scale
Linking Microstructural Evolution and Macro-Scale Friction Behavior in Metals
N. Argibay1, M. Chandross1,*, S. Cheng2, J.R. Michael1
1 Materials Science and Engineering Center, Sandia National Laboratories, Albuquerque, NM 87185 2 Department of Physics, Center for Soft Matter and Biological Physics and Macromolecules Innovation Institute, Virginia Polytechnic Institute and State University, Blacksburg, VA 24061 N. Argibay and M. Chandross contributed equally to this work. * Corresponding author e-mail address: email@example.com Abstract
A correlation is established between the macro-scale friction regimes of metals and a transition between two dominant atomistic mechanisms of deformation. Metals tend to exhibit bi-stable friction behavior -- low and converging or high and diverging. These general trends in behavior are shown to be largely explained using a simplified model based on grain size evolution, as a function of contact stress and temperature, and are demonstrated for pure copper and gold. Specifically, the low friction regime is linked to the formation of ultra-nanocrystalline surface films (10 to 20 nm), driving toward shear accommodation by grain boundary sliding. Above a critical combination of stress and temperature -- demonstrated to be a material property -- shear accommodation transitions to dislocation dominated plasticity and high friction. We utilize a combination of experimental and computational methods to develop and validate the proposed structure-property relationship. This quantitative framework provides a shift from phenomenological to mechanistic and predictive fundamental understanding of friction for crystalline materials, including engineering alloys.
Contrary to the centuries-old conventional wisdom that unlubricated self-mated pure metal contacts cold-weld, gall and invariably produce high friction and wear , we present evidence that it is in fact possible to achieve low friction (with friction coefficients of < 0.5) with pure bare metals such as pure Cu and Au. There are rare instances in the literature where this behavior has been shown before without surface modifying films, most prominently in Prasad et al.  for pure Ni and by Tamai for pure Cu and Au . More interestingly, pure metals exhibit an apparent bi-stability in their friction behavior, where in contact conditions associated with low friction the trends in friction appear to be converging, while the trends diverge for higher friction. Various authors [8, 1015] have reported that this unusual and highly desirable macro-scale behavior for pure metals and alloys are associated with the formation and persistence of a thin layer of highly refined, ultra-nanocrystalline (10 to 20 nm grain size) metal at the sliding surface, though the conditions and mechanism through which this layer is formed and how these two characteristics are correlated remains unclear. We propose a hypothesis and supporting evidence for a correlation between surface grain structure evolution and friction behavior of metals that is both predictive and quantitative, relying exclusively on materials properties and contact mechanics models to predict the bounds of observed friction regimes. The model is shown to accurately predict, without empiricism, the grain sizes of metal contacts in the low friction regime.
Central to the idea of a microstructural evolution model that drives metal friction behavior is the premise that the surface microstructure of a metal contact experiences a competition between grain refinement through plastic deformation and grain coarsening through grain boundary (GB) motion and dynamic
recrystallization. Be it through rolling[17, 18] or sliding[10, 11, 13, 14, 19, 20] there are many examples of grain refinement through cyclic contact via strain hardening, and more recently there are clear examples of coarsening of initially ultra-nanocrystalline metals[22, 23] as well as coarsening of more conventional fine-grained metal alloys[24, 25] toward an apparent stress-dependent equilibrium grain size. The idea that microstructural evolution and stability are the dominant characteristics of low friction behavior in bare metal sliding contacts is perhaps most clearly demonstrated by the electrical contacts community and literature in the form of noble metal alloys, primarily hard Au, as wear-resistant and low friction materials. With these alloys, the addition of as little as 0.1% by volume of an alloying species such as Ni or Co drastically reduces grain size and imparts astonishing wear resistance and low friction at contact stresses that would otherwise grossly deform pure Au[27, 28]. While recent work has shown that it is possible to achieve low friction and wear as well as electrical contact resistances indicative of bare metallic junctions using non-noble metals such as pure Cu in non-oxidizing environments[12, 2931], the advantages of relatively inert self-mated gold contacts as a baseline material are the reason why, in addition to Cu, it is one of the two material systems explored in this study.
As we show here, at sufficiently low applied stresses it is possible to achieve remarkably low friction ( < 0.5) with pure, coarse grained self-mated Au and even initially single crystal pure Cu, where severe galling and high friction ( > 1) would conventionally be expected to occur. While calling friction coefficients of < 0.5 low may seem to be excessively generous considering superlubricious materials such as graphene ( ~ 0.001) , for pure, bare metals sliding in inert environments it defies convention that the friction behavior should be anywhere below values commensurate with strong and rapid interfacial bonding. For pure, bare metals, the characteristic low friction regime appears to be associated with the formation and persistence of a stable nanocrystalline (NC) surface film [8, 11, 19], with grain sizes well below 100 nm. Similar to the formation of a Beilby layer  during metal polishing, we find that there is a well-defined stress and temperature regime where this highly refined surface layer can be made to persist. We calculate the limits of this regime for Cu and Au self-mated contacts and experimentally validate the predicted limits, by systematically varying contact stresses and temperatures. We propose a generalized model for FCC metals that allows prediction of three distinct friction regime boundaries (persistent low, transient and immediately high friction) in the space of stress, temperature and time, and demonstrate its validity for two FCC metals with significantly different properties. This model does not require empirical fitting and relies exclusively on well-defined materials properties (e.g. stacking fault energy, Burgers vector, and shear modulus), fundamental plasticity models (i.e. Yamakov et al. and van Swygenhoven et al.), and an appropriate contact mechanics model (e.g. Hamilton)[40, 41] used to determine the surface stress that drives grain size evolution. We chose the Hamilton contact model as there is a tractable and simple expression for the rapid calculation of maximum von Mises stress at the surface of a sphere-on-flat contact, which is shown to be a sufficiently accurate estimate of the stress driving surface grain growth in metal contacts that have been run-in.
As Johnson[17, 21] and Hamilton describe, at friction coefficients > 0.3 the location of maximum stress exists at the surface, which agrees well with the idea that these highly distorted ultra-nanocrystalline layers in metals should be present on the sliding surface for metal contacts. It is important to note that any calculation of maximum surface stress, such as that provided by Hamilton, is strongly dependent on the friction coefficient or surface shear stress. As a result, the determination of friction regimes as a function of surface stress, which is itself a function of friction coefficient, implies a feedback loop that can be either positive or negative. This feedback effect implies that the initial microstructure
does not necessarily dictate the steady-state friction behavior of a material. This idea agrees well with extensive data showing that it is possible to achieve low friction with initially coarse bare metal at sufficiently low contact stresses, and that a range of contact stresses ought to exist where transient and periodic behavior is observed, one of the three regimes identified as part of this model and demonstrated through experiments here with Au and Cu. We illustrate this feedback loop of stress, friction coefficient and grain size in Fig. 1A and the corresponding microstructural evolution model in Fig. 1B.
2. Materials, Experimental Methods and Characterization
The Au-Au contact consisted of a 1.59 mm radius spherically-tipped bulk hard gold alloy pin (Deringer-Ney Inc., Neyoro-G alloy) brought into sliding contact with a high purity (> 99.999 %) bulk gold ingot. Details of the pin composition and preparation are described elsewhere. The pure Au ingot was not polished to avoid transfer and embedding of hard particle media, instead it was pressed between polished W-C plates (average roughness, Ra < 20 nm) in a hydraulic press to 3 ksi pressure to achieve a smooth surface finish, yielding an average roughness Ra ~ 375 nm measured using a scanning white light interferometer (SWLI; Bruker Contour GT). The Cu-Cu contact consisted of a 1.19 mm radius UNS C10100 Cu ball bearing (McMaster-Carr) and a high purity (> 99.999 %) bulk single crystal substrate (Princeton Scientific, Princeton, NJ) with average surface roughness < 10 nm and an initial surface orientation of .
2.2 Friction Experimental Methods
The instrument used fo